Int. J. Electrochem. Sci., 7 (2012) 10627 - 10632
International Journal of
Improved Electrochemical Performance of LiMn2
Composite as Cathode Material for Lithium Ion Battery
Huayun Xu*, Bin Cheng, Yunpo Wang, Long Zheng, Xinhui Duan, Lihui Wang, Jian Yang, Yitai Qian Key Laboratory of the Colloid and Interface Chemistry (Shandong University), Ministry of Education, and School of Chemistry and Chemical Engineering, Shandong University, Jinan 250100, PR China *
Received: 26 September 2012 / Accepted: 13 October 2012 / Published: 1 November 2012
The electrochemical performance especially rate capability of LiMn2O4 is improved by graphene modified via ultrasonic agitation. The pristine LiMn2O4 and LiMn2O4/graphene composite are characterized by X-ray diffraction (XRD) and transmission electron microscopy (TEM). The obtained LiMn2O4/graphene composite shows reversible capacity of 107 mAh g-1 at 50 C charge/discharge rate. At 55 °C, the capacity at 5 C charge/discharge rate for LiMn2O4/graphene is higher than that of pristine LiMn2O4. The electrochemical impedance spectroscopy (EIS) indicates that the charge transfer resistance for LiMn2O4/graphene composite is reduced compared to LiMn2O4 sample.
Keywords: LiMn2O4/graphene; Rate capability; Lithium ion batteries; Composite materials; Sol-gel preparation
SM reported nanoscale LiMn2O4 (10-40 nm) with 27 wt% reduced graphene oxide hybrid as cathode material shows good rate capability . However, so high reduced graphene oxide content means a low volumetric capacity at high charge/discharge rate for their LMO/RGO sample.
In our study, LiMn2O4 (100 nm around) /graphene composite was tested as a cathode material for lithium ion battery, presenting high conductivity and good rate performance. A high energy density of 393 Wh kg-1 was obtained when charge/discharged at 50 C rate for 5 wt % graphene modified LiMn2O4 sample. Even at 55°C, discharge capacity of 97 mAh g-1 at 5C charge/discharge rate was maintained after 100 cycles for LiMn2O4/5 wt% G sample. The electrochemical impedance spectroscopy (EIS) indicated that the electrode impedance was decreased after modified graphene for LiMn2O4.
The LiMn2O4 was prepared by the sol–gel method using citric acid and glycol as the chelating agent. The stoichiometric amount of LiNO3 and 50 wt% Mn(NO3)2 solution were mixed with citric acid and glycol which their molar ratio was kept as 1:4 dissolved in 20 mL of distilled water. The molar ratio of metal ion to citric acid was 1:1. Then the solution was stirred at 80 °C for 2 h, and the obtained gel was dried at 180 °C for 10h. After that, it was sintered at 700 °C for 10 h. Graphene nanosheets, which were prepared by a chemical exfoliation process , were mixed with LiMn2O4 in ethanol solution with ultrasonic agitation and then sintered at 300 °C for 3h under argon atmosphere.
XRD patterns of the samples were provided using a Bruker D8 advanced X-ray diffractometer with Cu Kα radiation (λ=1.5418 Ǻ). The LiMn2O4/graphene composite was observed on a transmission electron microscope (TEM, JEOL-2010). The coin cells comprised of the prepared powder as cathode, lithium as anode, and an electrolyte having 1M LiPF6 in an ethylene carbonate (EC)-diethyl carbonate (DEC)-ethyl methyl carbonate (EMC) mixture (1:1:1). Micro-porous polypropylene separator was used in those cells. The cell preparation was carried out in an Ar-filled dry box. The charge/discharge cycles for assembled cells were measured using a Land CT2001 battery tester. EIS were performed by a Zahner Elektrik IM6 (Germany) impedance instrument over the frequency range of 100 kHz to 0.01Hz.
3. RESULTS AND DISCUSSION
3.1. Structure and morphology
space group of Fd3-m, except the peak at 2θ = 26.5° that can be assigned to the (002) plane of graphene sheets (Figure 1d). And this peak strengthens with the increase of graphene for LiMn2O4/G composite. Figure 2 shows the TEM image of (a) Graphene, (b) LiMn2O4, (c) LiMn2O4/2 wt% G and (d) LiMn2O4/5 wt% G. It can be seen that the particle size of LiMn2O4 is around ~ 100 nm (Figure 2b) and uniformly dispersed on the surface of graphene nanosheets as shown in Figure 2c and 2d.
Figure 1. XRD patterns of (a) LiMn2O4, (b) LiMn2O4/2 wt% G, (c) LiMn2O4/5 wt% G and (d) Graphene.
Figure 2. TEM of (a) Graphene, (b) LiMn2O4, (c) LiMn2O4/2%G, (d) LiMn2O4/5%G
3.2. Electrochemical Characterization
capability especially for LiMn2O4/5 wt % G sample which shows 107 mAh g-1 capacity when charged/discharged at 50 C rate, while only 80 mAh g-1 is obtained for pristine LiMn2O4 sample.
A higher rate performance was investigated for LiMn2O4/5 wt% G sample as given in Figure 3b. Even at 80 C charge/discharge rate, almost 60 mAh g-1 capacity is obtained. The charge/discharge curves for LiMn2O4/5 wt% G sample at different rate were shown in Fig. 3c. Seen from Figure 3d, the electrochemical performance of LiMn2O4/G is also improved compared to pristine LiMn2O4 sample at 55 °C. At 5C charge/discharge rate, about 97 mAh g-1 capacity after 100 cycles is maintained for LiMn2O4/5 wt% G, which is higher than that of pristine LiMn2O4. Yue synthesized LiMn2O4/C composite and obtained discharge capacity of 83 mAh g-1 at the current density of 2A g-1.Jia reported that they achieved LiMn2O4/CNT, which exhibited reversible capacity of 85 mAh g-1 at 1C . Liu also synthesized LiMn2O4/CNT by sol-gel route and discharge capacity of 31 mAh g-1 was achieved at the rate of 13 C. Bak synthesized LiMn2O4/RGO nanocomposite and reversible capacity of 101 mAh g-1 at 100 C was obtained. They found there was a large surface charge storage contribution for this good rate capability. Although the electrochemical property for LiMn2O4/5 wt% G sample in our work doesn’t exceed Bak’ result but it is comparable to Patey’s result, and, is superior to Yue, Jia and Liu’s reported results.
EIS was performed to investigate the electrode resistance changes for Li/LiMn2O4 and LiMn2O4/G samples as presented in Figure 4. The intercept at the real (Z’) axis in high frequency corresponds to the ohmic resistance (Re). The semicircle in the middle frequency range indicates the charge transfer resistance (Rct) and the inclined straight line relates to the Warburg impedance (Zw) . Seen from Fig. 4, the Rct value of the LiMn2O4, LiMn2O4/2 wt% G and LiMn2O4/5 wt% G sample is 165, 126 and 75 Ω, respectively. Clearly, the LiMn2O4/graphene sample can suppress the charge transfer resistance, which is contributed to a higher discharge capacity and high rate capability compared to the pristine LiMn2O4 sample (shown in Figure 3).
Figure 4. Nyquist plots of LiMn2O4, LiMn2O4/2 wt% G and LiMn2O4/5 wt% G samples
LiMn2O4 particles were modified by graphene nanosheets using ultrasonic agitation method. The obtained LiMn2O4/graphene composite performs a reversible capacity of 107 mAh g-1 at 50 C charge /discharge rate, The electrochemical properties of LiMn2O4/graphene composite at 55°C are also improved in this work. Greatly enhances of the electrical conductivity due to graphene and efficient use of the LiMn2O4, leading to an outstanding electrochemical performance of the hybrid cathodes.
1. J.B. Goodenough, and Y. Kim, Chem. Mater. 22 (2010) 587-603.
2. X.W. Li, R. Yang, B. Cheng, Q. Hao, H.Y. Xu, J. Yang, Y.T. Qian, Mater Lett, 66 (2012) 168-171.
3. A. Yamada, H. Koizumi, S.I. Nishimura, N. Sonoyama, R. Kanno, M. Yonemura, T. Nakamura, Y. Kobayashi, Nat. Mater. 5 (2006) 357-360.
4. Y.G. Wang, Y.R. Wang, E.J. Hosono, K.X. Wang, H.S. Zhou, Angew. Chem. Int. Ed. 47 (2008) 7461-7465.
5. Y. Zhou, J. Wang, Y. Hu, R.O. Hayreb, Z. Shao, Chem. Commun. 46 (2010) 7151-7153. 6. Y. Sharma, N.G. Sharma. V. Subba, B. Rao, V.R. Chowdari, Electrochim. Acta, 53 (2008)
7. Y. Wang, Z.S. Feng, J.J. Chen, Mater Lett, 71 (2012) 54-56.
8. X. Zhao, C.M. Hayner, H.H. Kung, J. Mater. Chem. 21 (2011) 17297- 17303.
9. S.M. Bak, K.W. Nam, C.W. Lee, K.H. Kim, H.C. Jung, X.Q. Yang, K.B. Kim, J. Mater. Chem. 21 (2011) 17309-17315.
10.X.F. Zhou, Z.P. Liu, Chem. Commun. 46 (2010) 2611-2613.
11.H. J. Yue, X. K. Huang, Do. P. Lv, Y. Yang. Electrochim. Acta, 54 (2009) 5363-5367. 12.X. L. Jia, C. Z. Yan, Z. Chen, Y. F. Lu. Chem. Commun., 47 (2011) 9669-9671. 13.X. M. Liu, Z. D. Huang, S. Oha. J. Power Sources, 195 (2010) 4290-4296.
14.S. M. Bak, K. W. Nam, C. W. Lee, K. B. Kim. J. Mater. Chem., 21 (2011) 17309- 17315.
15.T. J. Patey，R. Büchel, S. H. Nga, F. Krumeich, S. E. Pratsinis，P.Novák. J. Power Sources, 189 (2009) 149-154.